Skip to main content

Official Journal of the Japan Wood Research Society

# Calculation models of pressure and position of curved laminated veneer lumber in molds during pressing

## Abstract

Curved laminated veneer lumber (LVL) for use in furniture-making was produced from glue-coated pieces of rotary-cut veneers that were assembled and pressed between molds. Pressure was applied until glue-lines were set and finally held in an assembly of the desired curvature. Pressure was an important factor during pressing of curved LVL. In this study we deduced some equations for designing the shape of molds and calculating the total pressure from the mechanics. The results are summarized as follows: (1) The position angle of every section of curved LVL assembly in molds on the horizontal and the total pressure during pressing can be calculated in relation to the shapes and dimensions of the curved LVL. (2) The pressure distributions in the glue-line measured using pressure-sensitive film were in good agreement with the glue-line unit pressure provided for the experiment and calculation. Therefore, the equations deduced in this study were suitable for calculating the position angle and pressure of curved LVL in molds. (3) The total pressure on curved LVL was greater than the pressure on straight LVL. The total pressure consisted of the pressure on the glue-lines of straight LVL with the same length and width as curved LVL plus the supplementary pressure needed to bend the veneers. (4) The total pressures and position angles of curved LVL in molds were affected by the shape, bent angle, and length of each section of curved LVL.

## References

1. 1.

Wu ZH, Furuno T, Zhang BY (1998) Properties of curved laminated veneer lumber made from fast-growing species with radio frequency heating for use in furniture. J Wood Sci 44:275–281

2. 2.

Liu ZC, Zhang BY, Wu ZH (1989) Application and technology of bending and gluing multi-layer veneers in furniture manufacture. China For Prod Ind 3:25–28

3. 3.

Wu ZH, Furuno T, Zhang BY (1997) Temperature properties of curved laminated veneer lumber during hot pressing with radio frequency heating. Mokuzai Gakkaishi 43:847–854

4. 4.

Wu ZH (1989) Mold design and pressure calculation of laminated bends (in Chinese). Building Wood Based Panels 4:1119

5. 5.

Liu ZC (1983) Technology of wood products and furniture manufacture (in Chinese). China Forestry Publishing, Beijing, pp 239–250

6. 6.

Pound J (1966) Glue-line pressures. Wood (Nov):41–43

7. 7.

Pound J (1965) Making laminated shapes with RF heating. Wood (Oct):55–57

8. 8.

Kanamaru K (1965) Adhesion and lamination (in Japanese). Society of Polymer Science, Chijinshokan Co, Tokyo, pp 150–156

9. 9.

Itoh T, Maeda Y (1992) Strength of structures (in Japanese). Kokumin Kagaku, Tokyo, pp 1–13

10. 10.

Nagao H (1997) Industrial mechanics (in Japanese). Rikootosho, Tokyo, pp 11–48

11. 11.

Yang P, Hata M, Sasaki H, Konishi M, Oshiumi S (1991) Pressure distribution along glue-lines and bonding properties. I (in Japanese). Mokuzai Gakkaishi 37:611–618

12. 12.

Yang P, Hata M, Sasaki H (1991) Pressure distribution along gluelines and bonding properties. II (in Japanese). Mokuzai Gakkaishi 37:619–624

13. 13.

Pound J (1960) RF heating in chair manufacture. Wood (March):104–108

14. 14.

Pound J (1961) RF heating for shaped parts. Wood (Feb):50–60

Download references

## Author information

Authors

### Corresponding author

Correspondence to Zhi-Hui Wu.

## Rights and permissions

Reprints and Permissions

## About this article

### Cite this article

Wu, Z., Furuno, T. & Yoshihara, H. Calculation models of pressure and position of curved laminated veneer lumber in molds during pressing. J Wood Sci 45, 213–220 (1999). https://doi.org/10.1007/BF01177728

Download citation

• Received:

• Accepted:

• Published:

• Issue Date:

### Key words

• Curved LVL
• Mold
• Position angle
• Pressure